(2) ii. ©. 2016. Saurabh Bajaj All Rights Reserved.

(3) iii. I would like to dedicate the work that went into this thesis to my family and the support system at Caltech, including my advisor, G. Jeffrey Snyder..

(4) iv. Acknowledgements First and foremost, as clich´ed as it may sound, this work would really have not been possible without the support of my parents. They provided me with not only their hard-earned life savings to enable me to explore life and gain knowledge in this country, but also the emotional support and mental strength that I sought during many tough times.. I cannot thank my advisor, G. Jeffrey Snyder, enough for his support and patience with me while I explored how my interest and experience in computational thermodynamics and phase stability could be applied to the field of thermoelectric materials research. As he always maintained that his door is always open for students (so much so that he never set up appointment times with us), every one of my visits to his office filled me with motivation and encouragement. His enthusiasm for my projects (which was at times more than mine), technical expertise, and relentless pursuit for interesting science were critical in the coming about of this work. His extremely approachable and informal attitude, together with his ability to offer just about the right amount of guidance to his students (i.e., a balance between the extremes of hands-on and hands-off approaches) are qualities that not only proved to be beneficial, but according to me, are those of an ideal advisor.. The thermoelectric group members (most of whom have now graduated) are a great bunch of intellectuals full of fun and laughter, who are also very kind. I learned a lot about experimental techniques used in our labs from both Zachary Gibbs and Heng Wang, who patiently explained them to a novice like me. Zachary Gibbs also introduced me to the Materials Project (https://www.materialsproject.org/), and offered a lot of optimistic advice, both of which I am very grateful to him for. Gregory Pomrehn, and Jeff Doak and Christopher Wolverton of Northwestern University offered tremendous expertise and advice which was critical to my understanding of the.

(5) v complexity of defect physics.. Caltech goes out of the way to make students’ lives easier so that they have nothing else to worry about except academics, and I was a first-hand witness to this. Felicia Hunt and Natalie Gilmore of the Graduate Office, Maria Oh, Mariel Tourani, Charisma Bartlett, Alice Sogomonian, and Divina Bautista of the Health and Counseling Center are some of the many wonderful and critical members of the Caltech community who offered me immense support and encouragement throughout my years at Caltech.. The first few years at Caltech are generally pretty tough times for graduate students due to the burden of classes and preparation for qualifying/candidacy examinations, and I want to thank a few people who helped me make that time manageable. Nicolas Batara, my friend and colleague, spent a lot of the first year working together on problem sets. He is a gold mine of qualities, both personal and professional, that I admire and spent many lunches experiencing in awe. I am very thanful for what I have learned from them so far, and hope to continue to do so in the future. Gregory Atrian, mi amigo, not only gave me confidence during hard times, but always made him himself available to me for help when I needed it. He and I spent many weekends exploring Los Angeles and the vast amount of variety it offers in terms of cultures and cuisines. My friends, Lee Wilson and Pablo Guerrero, helped me escape the stresses of academic life with lots of laughter. Members of the MatSci lunch group including John Lloyd, Erik Verlage, and others provided for some entertaining times. I may have bothered Brent Fultz, one of my committee members, with an endless number of questions on the topics of entropy, thermodynamics, and kinetics, during/after his class and over email, but he patiently answered all of them to help me hold a strong grasp of the subjects.. I owe my mentors, Raymundo Arr¨oyave at Texas A&M University and Patrice Turchi at Lawrence Livermore National Laboratory, for all the support they provided to help propel me toward joining Caltech. Without them, I may not have reached this stage in my career, and I am grateful for their continued support. Sadasivan Shankar, who mentored me during my internship at Intel in the summer of 2013, taught me how to face and approach seemingly unsolvable and daunting problems, an invaluable skill. His guidance was vital to the nano phase diagram work described in this thesis, which I am very proud of..

(6) vi. A lot of my time at Caltech was spent swinging rackets in the recreational facilities at Caltech while playing tennis, squash, and most recently, UK (not US) racketball. These activities helped me keep sane and healthy, socialize, relieve stress, forget all my worries, and most importantly have fun and enjoy the times after work. None of them would be possible without the people who I played against: Evan Creer (tennis), Leslie Chill, Rob, Mark, Bob, Carl, Howard, Ronn, Eli Shechet (squash), and Eli Shechet (UK racketball) for introducing me to the great sport of UK racketball.. Last, but not the least, this work was supported by: Grants: EDCBEE under Contract No. DEAC02-05CH11231 (DOE), W31P4Q-13-1-0010 (DARPAARO), and NSC101-3113-P-008-001 (National Science Council of Taiwan). Computers: Chemical Engineering (CAT) Cluster at Texas A&M University; Hopper, Carver, and Mendel of National Energy Research Scientific Computing Center (NERSC) at Lawrence Berkeley National Laboratory; Wolf, Atom, and Ion of the Materials and Process Simulation Center (MSC) at Caltech. Internship opportunities: Intel Corporation, Robert Bosch RTC.

(7) vii. Abstract This thesis discusses the application of phase diagrams and the associated thermodynamics to semiconductor materials through theoretical computational calculations. The majority of work is focused on thermoelectric semiconducting materials that enable direct inter-conversion between electrical and thermal energy. First, one of the most efficient thermoelectric material, PbTe, is picked to demonstrate the assessment of unknown phase diagrams by combining two methods DFT and CALPHAD. Since there had been no previous investigations of defect stability in this material using computations, DFT is used to deduce the stability of various intrinsic point defects, and in turn attribute origins of n- and p-type conductivity to the most stable defects. Then, the calculated defect formation energies are used in the Pb-Te thermodynamic model built using the CALPHAD method to compare the estimated solubility lines and non-stoichiometric range of the PbTe phase with experimental data. Next, another lead chalcogenide, PbSe, is picked to explore the phase stability of the PbSe phase upon the addition of dopants (Br, Cl, I, Na, Sb, Bi, In), which is a common strategy to make thermoelectric materials and devices more efficient. The range of efficiencies and thermoelectric properties as functions of composition and temperature that can be achieved depends on the amount of dopant that can be added without precipitating secondary phases. Also, depending on the system and its phase diagram, there can be more than one way of doping a material. To help detail which method(s) of doping into PbSe will result in maximum dopant solubility, a procedure similar to the above for PbTe is followed by using DFT in combination with Boltzmann statistics to map solvus boundaries of the PbSe phase, but now in the ternary phase space of composition and temperature. This method also helps predict electrical conductivity, n- or p-type, in each region of the phase diagrams that represent different doping methods. Lastly, the role of surface energy contributions in changing phase stability at nano-dimensions.

(8) viii is explored. The CALPHAD approach is employed to investigate these changes in three systems by calculating their phase diagrams at nano dimensions and comparing them with their bulk counterparts..

(9) ix. Contents Acknowledgements. iv. Abstract. vii. 1 Introduction. 1. 1.1. Thermoelectric effect and applications . . . . . . . . . . . . . . . . . . . . . . . . . .. 1. 1.2. Motivation behind and organization of this thesis . . . . . . . . . . . . . . . . . . . .. 3. 2 Computational Methodology 2.1. 2.2. 8. Electronic structure calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 8. 2.1.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 8. 2.1.2. The Born-Oppenheimer Approximation . . . . . . . . . . . . . . . . . . . . .. 9. 2.1.3. Density Functional Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 10. 2.1.4. Kohn-Sham equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 10. 2.1.5. Generalized Gradient Approximation . . . . . . . . . . . . . . . . . . . . . . .. 12. 2.1.6. Solving the Kohn-Sham equations . . . . . . . . . . . . . . . . . . . . . . . .. 12. 2.1.7. Pseudo-potential method . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 12. The CALPHAD method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 13. 2.2.1. Ideal mixing. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 14. 2.2.2. Non-ideal mixing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 15. 2.2.3. Thermodynamic models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 16. 2.2.3.1. Random substitutional model . . . . . . . . . . . . . . . . . . . . . .. 16. 2.2.3.2. Sublattice model . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 17. 2.2.4. Evaluation of Gibbs energy parameters. . . . . . . . . . . . . . . . . . . . . .. 19.

(10) x 2.2.4.1. Minimization procedure for single-phase equilibria . . . . . . . . . .. 20. 2.2.4.2. Minimization procedure for two-phase equilibria . . . . . . . . . . .. 20. 2.2.4.3. Stepping and mapping . . . . . . . . . . . . . . . . . . . . . . . . . .. 22. 2.2.4.4. The PARROT programme . . . . . . . . . . . . . . . . . . . . . . .. 24. 3 Ab initio study of intrinsic point defects in PbTe: an insight into phase stability through defect thermodynamics. 26. 3.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 26. 3.2. Methodology . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 28. 3.2.1. Defect thermodynamics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 28. 3.2.2. Computational details . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 31. 3.2.3. Thermodynamic models for the CALPHAD method . . . . . . . . . . . . . .. 31. 3.2.3.1. Liquid . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 31. 3.2.3.2. PbTe . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 32. 3.2.3.3. Fcc A1, Hexagonal A8 . . . . . . . . . . . . . . . . . . . . . . . . .. 33. Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 34. 3.3.1. Defect stability . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 34. 3.3.2. Modification and assessment of the CALPHAD model . . . . . . . . . . . . .. 39. Conclusions and outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 41. 3.3. 3.4. 4 Calculation of dopant solubilities and phase diagrams of X-Pb-Se (X = Br, Na) limited to defects with localized charge. 45. 4.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 45. 4.2. Methodology . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 47. 4.2.1. Computational details . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 49. 4.3. Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 49. 4.4. Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 56. 5 Phase diagrams and defect thermodynamics to devise doping strategies in the thermoelectric material PbSe. 58. 5.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 58. 5.2. Methodology . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 60.

(11) xi. 5.3. 5.4. 5.2.1. Defect thermodynamics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 60. 5.2.2. Calculation of isothermal solvus boundaries . . . . . . . . . . . . . . . . . . .. 62. 5.2.3. Computational details . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 64. Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 65. 5.3.1. Cl, Br, and I in PbSe . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 65. 5.3.2. Sb and Bi in PbSe . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 69. 5.3.3. In in PbSe . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 74. Conclusions and outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 75. 6 Phase stability in nanoscale material systems: Extension from bulk phase diagrams. 80. 6.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 80. 6.2. Method and computational details . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 83. 6.2.1. The CALPHAD method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 83. 6.2.2. Extension of the CALPHAD method to nanoscale systems . . . . . . . . . . .. 84. 6.2.3. Assessment methodology. . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 89. 6.2.4. DFT calculations of surface energy . . . . . . . . . . . . . . . . . . . . . . . .. 90. Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 92. 6.3.1. Au-Si . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 92. 6.3.2. Ge-Si . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 95. 6.3.3. Al-Cu . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 97. Conclusions and outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 99. 6.3. 6.4. 7 Conclusions and summary. 106.

(12) xii. List of Figures 1.1. Contradictory nature of material properties that contribute to efficiency of thermoelectric materials plotted as functions of carrier concentrations. . . . . . . . . . . . . .. 1.2. 2. Schematic of a thermoelectric module with n-type and p-type legs connected electrically in series and thermally in parallel. As shown, the charge carriers travel from the hot side to the cold side, which drives a current I through the resistance R. . . . . . .. 2.1. 4. Schematic representation of random mixing of A and B atoms/molecules in a binary solution (adapted from Ref. [16]). . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 14. 2.2. Random occupation of sites on a bcc structure (adapted from Ref. [16]).. 16. 2.3. A bcc structure shown with preferential occupation of sites by atoms on the two simple cubic sublattices (adapted from Ref. [16]).. 2.4. . . . . . . .. . . . . . . . . . . . . . . . . . . . . . . . .. Schematic diagram showing the process of calculating the temperature at which ∆G1φ =0 (adapted from Ref. [16]). . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 2.5. 20. First stage in the iteration process of Gibbs energy minimization of a Cu-Ni alloy at composition x0 in Cu, and at 1523 K (adapted from Ref. [16]). . . . . . . . . . . . . . liq. 2.6. Gibbs energy versus N. 2.7. Calculation of the second derivative of G with respect to N liq to obtain the minimum. in an alloy shown schematically (adapted from Ref. [16]). .. in Gibbs energy (adapted from Ref. [16]). . . . . . . . . . . . . . . . . . . . . . . . . . 2.8. 17. 21 22. 23. Second, third, and fourth stage in the iteration process of Gibbs energy minimization of a Cu-Ni alloy with composition x0 in Cu, and at 1523 K (adapted from Ref. [16]). .. 24.

(13) xiii 3.1. (Color online) Calculated defect formation energies, ∆Hd,q in PbTe as a function of Fermi level, µe in Pb-rich and Te-rich conditions. Slope of lines corresponds to the charge state of the defect, and shaded areas represent the range of calculated equilibrium Fermi levels shown in Fig. 3.2. . . . . . . . . . . . . . . . . . . . . . . . .. 3.2. (Color online) Equilibrium positions of the Fermi level, µe for Pb-rich and Te-rich conditions obtained from solving the charge neutrality equation. . . . . . . . . . . . .. 3.3. 42. (Color online) Solidus lines of the PbTe phase calculated with the CALPHAD method compared with solubility lines calculated from DFT, and with experimental data.. 3.6. 39. (Color online) Pb-Te phase diagram calculated with the CALPHAD method and compared with experimental data. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 3.5. 38. (Color online) Calculated concentrations of electrons and holes for Pb-rich and Te-rich growth conditions, respectively, compared with experimental data from Refs. [31–35].. 3.4. 35. . .. 43. (Color online) Enthalpy of mixing of the liquid phase calculated at T = 1200 K with reference to the liquid phase states of Pb and Te, and compared with experimental data. 44. 3.7. (Color online) Chemical potential of Te in the liquid phase calculated at T = 1200 K with reference to the fcc phase of Pb and hexagonal phase of Te, and compared with experimental data. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 4.1. 44. (Color online) Defect formation energies, ∆Ed,q of the lowest energy intrinsic and Br-containing defects in PbSe as a function of Fermi level, µe (relative to VBM) in different three phase equilibrium regions of PbSe in the Br-Pb-Se phase diagram. Solid lines indicate defects included in the calculation of the Br-Pb-Se phase diagram, whereas dashed lines indicate excluded defects. . . . . . . . . . . . . . . . . . . . . . .. 4.2. 50. (Color online) Defect formation energies, ∆Ed,q of the lowest energy intrinsic and Na-containing defects in PbSe as a function of Fermi level, µe (relative to VBM) in different three phase equilibrium regions of PbSe in the Na-Pb-Se phase diagram. Solid lines indicate defects included in the calculation of the Na-Pb-Se phase diagram, whereas dashed lines indicate excluded defects. . . . . . . . . . . . . . . . . . . . . . .. 51.

(14) xiv 4.3. (Color online) Doping effectiveness of the shown defects at 973 K in the Pb-PbSePbBr2 region of Br-Pb-Se and PbSe-Na2 Se-NaSe region of Na-Pb-Se calculated by 0 varying the formation energies of the neutral BrSe and N a0P b defects (x-axis), respecT tively. ∆E - ∆EDF indicates the change from the true DFT calculated formation d,q. energy. Dashed lines mark the experimentally measured values of doping effectiveness for each system. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4. 54. (Color online) Partial charge density plot of the highest energy electrons in the su0 percell (of the PbSe primitive cell) containing the BrSe defect (at the center of the. supercell) showing charge delocalization that makes this defect equivalent to the case +1 of the charged defect BrSe with the Fermi level located at or near the CBM. Pb atoms. are shown in dark grey, Se atoms in light grey, and Br atom in green. . . . . . . . . . 4.5. 55. (Color online) (a) Isothermal section of the Br-Pb-Se phase diagram calculated at T = 973 K showing the single-phase region of PbSe in blue, and green tie-lines representing two-phase regions between it and other compounds that are shown in the full isothermal section plot in (b). Sample composition at which doping effectiveness measurements were made is shown as a closed blue circle in (a). Dashed line represents a path between PbSe and a hypothetical PbBr compound for one-to-one replacement of Se with Br, i.e., as PbBrx Se1−x . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 4.6. 56. (Color online) (a) Isothermal section of the Na-Pb-Se phase diagram calculated at T = 973 K showing the single-phase region of PbSe in blue, and green tie-lines representing two-phase regions between it and other compounds that are shown in the full isothermal section plot in (b). Sample composition at which doping effectiveness measurements were made is shown as a closed red circle in (a). . . . . . . . . . . . . .. 5.1. 57. (Color online) Defect formation energies, ∆Ed,q of the lowest energy intrinsic and Clcontaining defects in PbSe as a function of Fermi level, µe (relative to VBM) in different three phase equilibrium regions of PbSe in the Cl-Pb-Se phase diagram. Solid lines indicate defects included in the calculation of the Cl-Pb-Se phase diagram, whereas dashed lines indicate excluded defects. . . . . . . . . . . . . . . . . . . . . . . . . . . .. 66.

(15) xv 5.2. (Color online) Defect formation energies, ∆Ed,q of the lowest energy intrinsic and I-containing defects in PbSe as a function of Fermi level, µe (relative to VBM) in different three phase equilibrium regions of PbSe in the I-Pb-Se phase diagram. Solid lines indicate defects included in the calculation of the I-Pb-Se phase diagram, whereas dashed lines indicate excluded defects. . . . . . . . . . . . . . . . . . . . . . . . . . . .. 5.3. 67. (Color online) (a) Isothermal section of the Cl-Pb-Se phase diagram calculated at T = 573 K showing the single-phase region of PbSe in blue, and green tie-lines representing two-phase regions between it and other compounds that are shown in the full isothermal section plot in (b). Dashed line represents a path between PbSe and a hypothetical PbCl compound for one-to-one replacement of Se with Cl, i.e., as PbClx Se1−x . Point A (blue circle) marks the point of maximum Cl solubility in the three-phase region Pb-PbSe-PbCl2 where a sample is predicted to exhibit n-type conductivity, whereas point B (red circle) marks the point of Cl solubility in the three-phase region PbSe-Se-PbCl2 where a sample is predicted to exhibit p-type conductivity. . . . . . .. 5.4. 69. (Color online) (a) Isothermal section of the I-Pb-Se phase diagram calculated at T = 573 K showing the single-phase region of PbSe in blue, and green tie-lines representing two-phase regions between it and other compounds that are shown in the full isothermal section plot in (b). Dashed line represents a path between PbSe and a hypothetical PbI compound for one-to-one replacement of Se with I, i.e., as PbIx Se1−x . Point A (blue circle) marks the point of maximum I solubility in the three-phase region Pb-PbSe-PbI2 where a sample is predicted to exhibit n-type conductivity, whereas point B (red circle) marks the point of I solubility in the three-phase region PbSe-SePbI2 where a sample is predicted to exhibit p-type conductivity. . . . . . . . . . . . .. 70.

(16) xvi 5.5. (Color online) (a) Isothermal section of the Br-Pb-Se phase diagram calculated at T = 573 K showing the single-phase region of PbSe in blue, and green tie-lines representing two-phase regions between it and other compounds that are shown in the full isothermal section plot in (b). Dashed line represents a path between PbSe and a hypothetical PbBr compound for one-to-one replacement of Se with Br, i.e., as PbBrx Se1−x . Point A (blue circle) marks the point of maximum Br solubility in the three-phase region Pb-PbSe-PbBr2 where a sample is predicted to exhibit n-type conductivity, whereas point B (red circle) marks the point of Br solubility in the threephase region PbSe-Se-PbBr2 where a sample is predicted to exhibit p-type conductivity. 71. 5.6. (Color online) Defect formation energies, ∆Ed,q of the lowest energy intrinsic and Sb-containing defects in PbSe as a function of Fermi level, µe (relative to VBM) in different three phase equilibrium regions of PbSe in the Sb-Pb-Se phase diagram. Solid lines indicate defects included in the calculation of the Sb-Pb-Se phase diagram, whereas dashed lines indicate excluded defects. . . . . . . . . . . . . . . . . . . . . . .. 5.7. 72. (Color online) Defect formation energies, ∆Ed,q of the lowest energy intrinsic and Bicontaining defects in PbSe as a function of Fermi level, µe (relative to VBM) in different three phase equilibrium regions of PbSe in the Bi-Pb-Se phase diagram. Solid lines indicate defects included in the calculation of the Bi-Pb-Se phase diagram, whereas dashed lines indicate excluded defects. . . . . . . . . . . . . . . . . . . . . . . . . . . .. 5.8. 73. (Color online) (a) Isothermal section of the Sb-Pb-Se phase diagram calculated at T = 573 K showing the single-phase region of PbSe in blue, and green tie-lines representing two-phase regions between it and other compounds that are shown in the full isothermal section plot in (b). Dashed line represents a path between PbSe and a hypothetical SbSe compound for one-to-one replacement of Pb with Sb, i.e., as Pb1−x Sbx Se. Point B (blue circle) marks the point of maximum Sb solubility in the three-phase region PbSe-Sb-Sb2 Se3 where a sample is predicted to exhibit n-type conductivity, whereas point C (red circle) marks the point of Sb solubility in the threephase region PbSe-Sb2 Se3 -Se where a sample is predicted to exhibit p-type conductivity. 75.

(17) xvii 5.9. (Color online) (a) Isothermal section of the Bi-Pb-Se phase diagram calculated at T = 573 K showing the single-phase region of PbSe in blue, and green tie-lines representing two-phase regions between it and other compounds that are shown in the full isothermal section plot in (b). Dashed line represents a path between PbSe and a hypothetical BiSe compound for one-to-one replacement of Pb with Bi, i.e., as Pb1−x Bix Se. Point B (blue circle) marks the point of maximum Bi solubility in the three-phase region PbSe-Bi-Bi2 Se3 where a sample is predicted to exhibit n-type conductivity, whereas point C (red circle) marks the point of Bi solubility in the three-phase region PbSe-Bi2 Se3 -Se where a sample is predicted to exhibit p-type conductivity. . . . . . .. 5.10. 76. (Color online) Defect formation energies, ∆Ed,q of the lowest energy intrinsic and Incontaining defects in PbSe as a function of Fermi level, µe (relative to VBM) in different three phase equilibrium regions of PbSe in the In-Pb-Se phase diagram. Solid lines indicate defects included in the calculation of the In-Pb-Se phase diagram, whereas dashed lines indicate excluded defects. . . . . . . . . . . . . . . . . . . . . . . . . . . .. 5.11. 78. (Color online) (a) Isothermal section of the In-Pb-Se phase diagram calculated at T = 573 K showing the single-phase region of PbSe in blue, and green tie-lines representing two-phase regions between it and other compounds that are shown in the full isothermal section plot in (b). Point C (blue circle) marks the point of maximum In solubility in the three-phase region PbSe-InSe-In2 Se3 where a sample is predicted to exhibit n-type conductivity, whereas point D (red circle) marks the point of In solubility in the three-phase region PbSe-In2 Se3 -Se where a sample is predicted to exhibit p-type conductivity. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 6.1. 79. (Color online) Phase diagram of the Ge-Si alloy system calculated for two particle shapes - sphere and a regular icosahedron, both for a particle size of 5 nm, and compared with the bulk phase diagram.. 6.2. . . . . . . . . . . . . . . . . . . . . . . . . .. 86. (Color online) Calculated melting points of Au as a function of particle size compared with experimental data from Ref. [179]. . . . . . . . . . . . . . . . . . . . . . . . . . .. 94.

(18) xviii 6.3. (Color online) Calculated melting points of Si, using surface tension data from Mallot et al [151] for liquid and from Jaccodine et al [152] for the solid phase, as a function of particle size compared with experimental data from Iida & Guthrie [153], Mezey et al [158], Couchman & Jesser [170], Buffat & Borell [180], and Goldstein [171]. . . . . .. 6.4. 95. (Color online) Au-Si phase diagram. (a) Phase diagram of the Au-Si alloy system calculated for particles of radius, r = 7 nm, and compared with the bulk phase diagram from Ref. [174]. (b) Part of Au-Si phase diagram showing the amounts of shift in solubility lines which agrees well with experimental results from Ref. [132] shown in parentheses. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 6.5. 96. (Color online) Ge-Si phase diagram. (a) Bulk Ge-Si phase diagram calculated using data from Refs. [26, 175, 176]. (b) Phase diagram of the Ge-Si alloy system calculated for varying radii particles, and compared with the bulk phase diagram. With decreasing particle radii, the peak temperature of the miscibility gap decreases from ≈ 226 K for bulk particles to ≈ 68 K for particles of radii, r = 5 nm.. 6.6. . . . . . . . . .. 97. (Color online) Calculated surface tension of the liquid phase in the Ge-Si system compared with experimental data from Ref. [177]. Dashed line only serves as a guide to the eye. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 6.7. (Color online) Calculated melting points of Ge as a function of particle size compared with experimental data from Ref. [181]. . . . . . . . . . . . . . . . . . . . . . . . . . .. 6.8. 98. 99. (Color online) Al-Cu phase diagram. (a) Bulk Al-Cu phase diagram according to Refs. [163, 164]. (b) Phase diagram of the Al-Cu alloy system calculated for particles of radius r = 10 nm, compared with the bulk phase diagram at Al-rich/Cu-poor compositions. The eutectic temperature drops from ≈ 821 K for bulk particles to ≈ 695 K for particles of radii, r = 5 nm. . . . . . . . . . . . . . . . . . . . . . . . . . . . 100. 6.9. (Color online) Unit cell of the Al2 Cu compound. . . . . . . . . . . . . . . . . . . . . . 101.

(19) xix 6.10. (Color online) Slab models created for the calculation of surface energies of the (100), (110), and (111) planes in the Al2 Cu compound. These surface energies can then be used to calculate the surface energy contribution to the total Gibbs free energy of this phase, which will lead to the estimation of the change in phase stability of this compound in the phase diagram as a function of particle radii. Since the surface energy can theoretically be calculated for any compound using DFT, this method can be applied to all the phases in a system including equilibrium, metastable, and unstable phases. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 102. 6.11. (Color online) Calculated melting points of Al as a function of particle size compared with experimental data from Ref. [185]. . . . . . . . . . . . . . . . . . . . . . . . . . . 102. 6.12. (Color online) Calculated melting points of Cu as a function of particle size compared with experimental data from Ref. [186]. . . . . . . . . . . . . . . . . . . . . . . . . . . 105. 6.13. (Color online) Calculated surface tension of the liquid phase in the Al-Cu system compared with experimental data from Refs. [156, 187]. . . . . . . . . . . . . . . . . . 105.

(20) xx. List of Tables 3.1. Defect formation energies ∆Hd,q (eV/defect) calculated for each point defect considered in the PbTe system for chemical potentials corresponding to Pb-rich and Te-rich conditions. Values are determined at µe = 0.42 eV for Pb-rich and µe = 0.31 eV for Te-rich conditions, which are the equilibrium Fermi levels (relative to the VBM) obtained at T = 300 K by solving the charge neutrality equation, as shown in Fig. 3.2. Only the lowest energy charge state for each defect at this Fermi level, corresponding to Fig. 3.1, is shown.. 3.2. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 38. Model description and parameters for phases in the Pb-Te system. The functions GHSERPB, GHSERTE, GLIQPB, and GLIQTE are obtained from the SGTE database [26]. Parameters X2 and X3 in the Gibbs free energy expansion of the PbTe phase shown in Eqn. (3.10) are fixed to the DFT defect formation energies of VT+2 e and VP−2 b defects, respectively, shown in Table 3.1 and as explained in Section 3.3.2. Thus, X2 = 0.72 eV/defect = 69,469 J/mol, and X3 = 0.35 eV/defect = 33770 J/mol, as listed below. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 41. 6.1. Surface area to volume ratio of different shapes of nano-particles. . . . . . . . . . . . .. 82. 6.2. Thermodynamic and physical properties used in the calculation of alloy surface tensions and phase diagrams of the Au-Si, Ge-Si, and Al-Cu nanoscale systems (L: Liquid, S: Solid) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 91.

(21) xxi 6.3. Thermodynamic functions used in the calculation of phase diagrams in this work (in J mol−1 and K). All bulk and size-independent functions are obtained from (a) Au-Si: SGTE database [26] and Ref. [174], (b) Ge-Si: SGTE database [26] and Refs. [175] and [176] for the liquid and diamond phases, respectively, and (c) Al-Cu: Ref. [164] for the liquid and γD83 phases, and the COST-507 database [163] for the rest of the phases. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 103. 6.4. Change in points on the phase diagram for particles from bulk to nanoscale dimensions. Au-Si: temperature and composition of the eutectic point - Liq → fcc-Au + dia-Si, Ge-Si: peak temperature of the miscibility gap in the diamond phase, and Al-Cu: temperature and composition of the eutectic point - Liq → fcc-Al + Al2 Cu. . . . . . . 104. 6.5. Calculated lattice constants (in ˚ A) and cohesive energy, Ecoh (in eV/atom) of Al, Cu, and the Al2 Cu phase from DFT using the LDA approximation. Experimental data are shown in parentheses. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 104. 6.6. Converged surface tension values of different planes in the Al2 Cu intermetallic compound calculated from DFT using the LDA approximation. . . . . . . . . . . . . . . . 104.

(22) 1. Chapter 1. Introduction 1.1. Thermoelectric effect and applications. The effect of climate change and global warming in raising earth’s average temperature is undeniable considering the available evidence [1, 2]. The rise in temperature will have detrimental effects on the current state of social and economic life. There have been several cycles of glacial advance and retreat in this time period; however, the current trend of glacial melting due to the highest levels of carbon dioxide in the atmosphere in 650,000 years is unprecedented. More importantly, 97% of the scientific community is in robust consensus that this effect is anthropogenic-based [3–5]. Thus, the need for renewable energy technologies such as wind, solar, etc. that do not release greenhouse gases to the atmosphere is urgent, and it is widely agreed that the energy source portfolio of the future will be a mix of these technologies rather than being dominated by one single source.. Waste heat recovery using thermoelectric generators is one such technology that is expected to play an important role in the formation of an energy portfolio, especially considering that somewhere between 20 to 50% of industrial energy input is lost as waste heat in the form of hot exhaust gases, cooling water, and heat lost from hot equipment surfaces and heated products [6]. Thermoelectric materials have already found applications in a wide variety of applications, such as a replacement of alternators in automobiles to directly convert waste exhaust heat to electric power [7, 8], and in radioisotope thermoelectric generator to power space rovers [9, 10], etc. Thermoelectric devices have many advantages over heat engines, such as having spot temperature control and being low maintenance, and, as they are solid-state devices, they have no moving parts, thus.

(23) 2 making their operation quiet and vibration free. These advantages enable its application for remote sensing, such as in the Voyager spacecrafts of NASA-JPL, which has been one of its most prolific and successful applications [11]. These deep space probes, after a journey of more than 37 years, have reached interstellar space, the furthest point any man-made object has reached, which proves power stability of thermoelectric devices over extended periods of time.. To be able to convert energy from heat into electrical voltage and vice-versa, the material needs to contain free charge carriers to make this energy transfer possible. It is also desirable that it have high electrical conductivity while maintaining a low thermal conductivity so that charge carriers can be transported without compromising temperature gradient. These characteristics are interdependent on each other and on carrier concentrations, as can be seen from Fig. 1.1.. Figure 1.1: Contradictory nature of material properties that contribute to efficiency of thermoelectric materials plotted as functions of carrier concentrations. The efficiency of thermoelectric materials is measured by the figure of merit zT , which is given by,.

(24) 3. zT =. S 2 σT , (κL + κe ). (1.1). where, S is the Seebeck coefficient, σ is the electrical conductivity, T is the absolute temperature, and κL and κe are the lattice and electronic thermal conductivities, respectively. To maximize zT , a large Seebeck coefficient is needed, which is ensured when only a single type of carrier (electrons or holes) is present in the material, while also maximizing electrical conductivity and minimizing thermal conductivity. As can be seen from Fig. 1.1, zT commonly peaks at carrier concentrations of 1018 to 1021 carriers/cm3 . Such carrier concentrations are typical of low band gap heavily doped semiconductor materials that fall in a domain between metals and conventional semiconductors. The thermoelectric effect is based on three correlated effects: the Seebeck effect, the Peltier effect and the Thomson effect. The Seebeck effect, named after Thomas Johann Seebeck who discovered it in 1822, is most often discussed when characterizing thermoelectric performances, as in practice, the Seebeck effect is most convenient with respect to lab measurements of voltage generated per degree of temperature difference. According to this effect, when one side of the material is heated while the other side is kept cooler, electrons diffuse to the cold side of the material. This phenomenon is schematically shown in Fig. 1.2 in a thermoelectric module consisting of one n-type and one p-type leg that are electrically connected in series and thermally in parallel. To balance this chemical diffusive driving force created by a temperature gradient, a stable electric field/voltage is generated across the material to drive a current I through the resistance R.. 1.2. Motivation behind and organization of this thesis. The stumbling block that has kept thermoelectric devices out of widespread commercial applications is their low Carnot efficiency compared with heat engines and their economic evaluations [12]. One of the factors contributing to these low efficiencies occurs at the contacts between source and device in maintaining a steady thermal transfer, but another major contributing factor arises from the efficiency of the material itself. The latter has been subject of the majority of thermoelectric materials research.. The lead chalcogenides (PbQ, Q = Te, Se, S) crystalize in a cubic rock salt structure with space.

(25) 4. Cold side. Figure 1.2: Schematic of a thermoelectric module with n-type and p-type legs connected electrically in series and thermally in parallel. As shown, the charge carriers travel from the hot side to the cold side, which drives a current I through the resistance R. group Fm3m (no. 225), and are one of the most well studied class of thermoelectric materials due to their highly symmetric structure, relatively simple defect chemistry, and ease of synthesis without competing phases. They also have the advantages of have narrow band gaps with fairly high carrier mobilities, and their carrier densities are easily tunable between the ranges of 1016 to 1021 carriers/cm3 for both n- and p-type operation, thus making them ideal for thermoelectric and optoelectronic applications. PbTe based alloys used in thermoelectric generators have a peak zT of around 0.8 for both n- and p-type operation [13]. The bulk of the work in this thesis is focused on two such lead chalcogenides, PbTe, and its less studied analog, PbSe.. Defect control is critical in semiconductors and a prerequisite to optimize zT not only because intrinsic defects and intentional doping is a primary means of controlling the majority carrier type for charge transport, but also because defects can significantly alter properties of semiconductors. This is challenging and in many cases has impeded the realization of the best zT as predicted. Thus, first in Chapter 3, the stability of intrinsic point defects in PbTe, one of the most widely studied and efficient thermoelectric material, is explored by means of Ab initio based Density Functional Theory (DFT) [14, 15], a method that is described in detail in Chapter 2. Prior to this work, to the author’s knowledge, there was no study on intrinsic point defects in PbTe, making this work.

(26) 5 even more critical. These calculations could prove to be very helpful in determining the defect thermodynamics of various defects in this system. The origin of n- and p-type conductivity in PbTe is attributed to particular intrinsic charged defects by calculating their formation energies. These DFT calculated defect formation energies are then used in the Gibbs free energy description of this phase as part of the Pb-Te thermodynamic model built using the CALPHAD (CALculation of PHAse Diagrams) approach [16] (also described in detail in Chapter 2), and in the resulting phase diagram it is found that its solubility lines and non-stoichiometric range agree very well with experimental data. Such an approach of using DFT in conjunction with CALPHAD for compound semiconductor phases that exhibit very small ranges of non-stoichiometry does not only make the process of calculating phase diagrams for such systems more physical, but is necessary and critical for the assessment of unknown phase diagrams. A CALPHAD type thermodynamic model is necessary to improve our understanding of phase stability, phase equilibrium, and thermodynamics for a system. Chapter 3 presents the methodology and approach of the CALPHAD technique which involves the modeling of Gibbs energies of all the phases taking part in equilibrium through reliable and consistent experimental data. Such a model offers many advantages: (i) it can be extrapolated to regions of temperatures and compositions which are not easily accessible by experiments, (ii) and it provides an easy way to study how equilibria and reactions are affected by various external factors. The use of such techniques plays an even more important role since experiments are challenging and expensive for this class of systems.. For additional control over the performance of a semiconductor for a specific application, an external dopant is usually added to it which allows for precise control over electron and hole densities, which in turn is directly related to the dopant concentration. It is an essential strategy to improve the efficiency of thermoelectric materials and devices. Thermoelectric semiconductors are so heavily doped that their transport properties mimic properties of metals more than semiconductors. The doping levels in these materials are orders of magnitude higher than in other semiconductors, making intrinsic impurities or self-doping less important than extrinsic impurities. To estimate the amount of dopant that can be added to a semiconductor without precipitating secondary phases, a detailed phase diagram is needed. Calculated phase diagrams could be very helpful when time-consuming experimental ones are not available. In Chapter 4, we have calculated dopant solubilities of Br and Na in the thermoelectric material PbSe by mapping its solvus.

(27) 6 boundaries in different regions of the respective ternary phase diagrams using DFT defect energy calculations. The narrow gap PbSe provides an example where most defects with charge state as expected from electron count are properly localized, whereas other charge states of defects lead to charge delocalization, which, in effect, alter their charge state to those of localized defects. The equilibrium electron chemical potential is positioned where the defect landscape is dominated by delocalized defects that, from the view of defect thermodynamics, are not expected to be stable or play a role in controlling the majority carrier type or concentration, resulting in unexpected dopant concentrations and solubilities. Experimentally measured doping efficiencies for these systems indicate much higher formation energies for these defects, beyond the inaccuracies of the calculations due to any known reason. Performing thermodynamic calculations using only the expected charge states, precluding others, enables accurate prediction of experimentally measured doping efficiencies and phase diagrams. Utilizing such a method in related semiconductors containing only localized defects will expedite the use of such calculations by experimentalists in understanding phase diagrams and devising effective doping strategies.. Cl, Br, I, Sb, Bi, and In are popular n-type and p-type dopants in PbSe and other chalcogenides. The range of thermoelectric properties as a function of carrier concentration and temperature, such as Seebeck coefficient and electrical conductivity, that can be achieved depends on the amount of dopant that can be added to it without precipitating secondary phases. This requires a mapping of solvus boundaries of the thermoelectric phase in composition and temperature space upon the addition of a dopant. In Chapter 5, we employ density functional theory (DFT) calculations to predict the most stable defects in different regions of thermodynamic phase stability between the PbSe phase and these dopants. When this information is used as input to a statistical mechanics model, we determine the dilute-limit single-phase boundary of PbSe in each ternary system containing the dopant. This enables the calculation of dopant solubility and carrier concentration in PbSe in the ternary composition space as a function of temperature, which helps detail which method(s) of doping into PbSe will result in maximum dopant solubility without precipitating second phases. As will be shown in this chapter, it also helps predict electrical conductivity behavior, electron or hole type, in each phase region representing the different doping methods.. Lastly, in Chapter 6, the effect of grain size of material alloys on their phase stability and phase.

(28) 7 diagrams is explored. Phase diagrams of multi-component systems are critical for the development and engineering of material alloys for all technological applications. At nano dimensions, surfaces (and interfaces) play a significant role in changing equilibrium thermodynamics and phase stability. In this work, it is shown that these surfaces at small dimensions affect the relative equilibrium thermodynamics of the different phases. The CALPHAD approach for material surfaces (also termed “nano-CALPHAD”) is employed to investigate these changes in three binary systems by calculating their phase diagrams at nano dimensions and comparing them with their bulk counterparts. The surface energy contribution, which is the dominant factor in causing these changes, is evaluated using the spherical particle approximation. Butler’s equations are used to calculate alloy surface tensions, which along with bulk thermodynamic models, are used to calculate interaction parameters to develop thermodynamic models. It is first validated with the Au-Si system for which experimental data on phase stability of spherical nano-sized particles is available, and then extended to calculate phase diagrams of similarly sized particles of Ge-Si and Al-Cu. Additionally, the surface energies of the associated compounds are calculated using DFT, and integrated into the thermodynamic model of the respective binary systems. Computed data on melting points of pure components, and alloy surface tensions are compared and agree well with available experimental data. In this work we found changes in miscibilities, reaction compositions of about 5 at.%, and solubility temperatures ranging from 100-200 K for particles of sizes 5 nm, indicating the importance of phase equilibrium analysis at nano dimensions.. Finally, a summary of the thesis is provided in Chapter 7, where it is explained how the results of this work on defect thermodynamics fit within the larger context of determining phase equilibria in binary and ternary multi-component thermoelectric alloys, and directions on future work that can be undertaken to achieve the objective of devising effective doping strategies will be briefly discussed..

(29) 8. Chapter 2. Computational Methodology 2.1 2.1.1. Electronic structure calculations Introduction. Density Functional Theory (DFT) has been one the most important breakthroughs in the physical sciences in the last 50 years, and is a popular method for the quantum mechanical solution of periodic systems to compute the electronic structure of matter. It has proven to be a very successful approach for the description of ground-state properties of metals, semiconductors, and insulators, and thus its application to study a large number of properties of real materials has seen an explosive growth over the last couple of decades, especially considering the exponential increase in supercomputing power. It is partly a parameterless method, which is why it is sometimes referred to as an ab inito method, and so its results are considered fundamental in a physical sense. The fundamental principle of DFT is that any property of a system consisting of many-body interactions can be viewed as a functional of the ground state density, which in principle, determines all information on the ground state. In this section, a succinct description of the formulation is described. A good exposition of the method can be found in Ref. [17].. Consider a solid of atomic number Z, and composed of N number of nuclei. These nuclei are positively charged particles and heavier than the negatively charged electrons. The total number of interacting particles in such a solid becomes (N + Z.N ), thus making this a many-body problem. The Hamiltonian for a solid is given by,.

(30) 9. 2. ˆ H. = −. 2 − − ¯h X ∇→ ¯h X ∇→ Ri ri − 2 i Mi 2 i me. 1 X e2 Zi 1 X e2 + − − − − 4π0 i,j | → 8π0 |→ ri − → rj | Ri − → rj | i 6= j 1 X e2 Zi Zj + → − → − 8π0 i 6= j | R i − R j |. −. (2.1). − → − where the nuclei are of mass Mi and at Ri , and the electrons are of mass me and at positions → ri . The charge of the electron is e. The first two terms are the kinetic energy operators of the nuclei and electrons, respectively. The last three terms describe the Coulombic interactions between a nucleus and an electron, between two electrons, and between two nuclei, respectively.. Even for the modern-day computers, it is extremely challenging to solve Eqn. (2.1) exactly for elements with more than a few electrons. Thus, several approximations are made to ease the calculations. These are briefly described in the following subsections.. 2.1.2. The Born-Oppenheimer Approximation. This approximation, also known as the adiabatic approximation, assumes the nuclei to be “frozen” due to their heavier masses. Thus, the kinetic energy term of the nuclei is eliminated, and the potential term now becomes a constant. Thus, only electrons are left as interacting particles in this many-body problem, and Eqn. (2.1) reduces to ˆ = Tˆ + Vˆ + Vˆext , H. (2.2). where the first term (Tˆ) is the kinetic energy operator for the electrons, the second term (Vˆ ) describes the potential energy between the electrons, and the last term (Vˆext ) is the potential energy of the electrons in the external potential of nuclei..

(31) 10. 2.1.3. Density Functional Theory. After the first level of approximation, the problem becomes simpler, but still remains difficult to ˆ is still intractable for systems with more than a few dozen atoms because solve; the solution of H the many-body wave function depends on at least 3N variables for a system with N interacting electrons. Thus, the so-called Density Functional Theory (DFT) is used to simplify the problem further and this method relies on two important theorems by Hohenberg and Kohn [14]. The first theorem states that there is a one-to-one relationship between the external potential Vext and the − ground-state density ρ(→ r ) of a many-electron system. The Hamiltonian is determined by Vext , − so all the properties of the many particle system follow from a specification of ρ(→ r ). The second − theorem states that the lowest energy is obtained if and only if the ground state density ρ0 (→ r ) is used in the energy functional. It establishes a variational principle for the ground-state total energy functional H[ρ] ≡ EVext [ρ] as, EVext [ρ] = < ψ|Tˆ + Vˆ |ψ > + < ψ|Vˆext |ψ >, | {z }. (2.3). FHK [ρ]. where the Hohenberg-Kohn density functional FHK [ρ] is universal for many-electron systems as it contains information regarding only electrons and not protons. It is postulated in this theorem that at the ground-state density Vext , the ground-state energy functional EVext [ρ] reaches its minimum value.. 2.1.4. Kohn-Sham equations. The Kohn-Sham equations helped turn DFT into a usable and practical tool. The first formulation is defined for the correlation energy, which is the part of the total energy present in the exact solution, but absent in the Hartree-Fock solution, and is given by,. Vc = T − T0 ,. (2.4). where T is the exact kinetic energy functional for the electrons, and T0 is the kinetic energy functional for a non-interacting electron gas. The second formulation defines the exchange contribution to the total energy that is present in the Hartree-Fock solution, and absent in the Hartree solution. Thus, it is given by,.

(32) 11. Vx = V − VH ,. (2.5). where V is the exact electron-electron potential energy functional, and VH is the Hartree contribution. Thus, the Hohenberg-Kohn functional, from Eqn. (2.3) is written in the following way:. FHK. =. T0 + V + (T − T0 ). = T0 + V + Vc. f rom (2.4). =. f rom (2.5),. T0 + VH + Vc + Vx. where Vxc is the exchange-correlation energy functional. The energy functional is thus written as,. EVext [ρ] = T0 [ρ] + VH [ρ] + Vxc [ρ] + Vext [ρ].. (2.6). The corresponding Kohn-Sham Hamiltonian is given by, ˆ KS = Tˆ0 + VˆH + Vˆxc + Vˆext . H. (2.7). For a system with N particles, the Hamiltonian is solved as a one particle system in its N lowest eigenstates φi , usually referred to as the Kohn-Sham orbitals. The eigenstates are then determined by solving a Schr¨ odinger-like non-interacting single-particle equation given by, ˆ KS φi = i φi . H. (2.8). These N equations are the Kohn-Sham equations, and are at the heart of DFT. They can be solved by expanding the single electron wave functions in a basis and diagonalizing the Hamiltonian − matrix. Since both V and V depend on the electron density ρ(→ r ), which in turn depends on H. xc. the wavefunctions φi being calculated, this problem becomes self-consistent. In the first step, an initial guess of the electron density density ρ0 is made. With this value, the Hartree operator VH and exchange-correlation operator Vxc , both of which depend on ρ0 , are calculated. Thus, the Hamiltonian HKS is constructed, and the eigenvalue problem is solved to obtain φi which in turn leads to the calculation of a new density ρ1 . This new density is then compared with the starting.

(33) 12 guess ρ0 , and the procedure is repeated again until both become equal.. 2.1.5. Generalized Gradient Approximation. This approximation method for the exchange-correlation functional is used for the work presented in this thesis. In this method, the exchange-correlation contribution of every infinitesimal volume not only depends on that volume, but also on the density in neighboring volumes [18]. Thus, the gradient in density between different volumes is also taken into account, and thus it is termed as Generalized Gradient Approximation (GGA).. 2.1.6. Solving the Kohn-Sham equations. The single-electron equations to solve are infinite and similar to Eqn. (2.8) irrespective of the method of approximation chosen for the exchange-correlation functional. The wave functions are expressed as,. φm =. P X. b cm p φp ,. (2.9). p=1 b where cm p are the coefficients to be calculated, and φp is a basis set. The dimensions of the function. space in which the wave functions φm are being searched, are infinite, thus making P infinite. However, it is impossible to work with an infinite basis set, and thus its selection is made in such a way that the resulting functions are close to φm . The larger the value of P , the more accurate the wave functions, but more time consuming the calculations. Once the selection of a basis set is made, solving Eqn. (2.8) becomes an eigenvalue problem. The choice of a basis set is made in such a way that it is both efficient, i.e., it represents the wave functions as closely as possible, thus requiring lower values of P , and unbiased, i.e., its properties are not influenced by the wave functions. One such basis set that satisfies both of these requirements quite well is the plane wave basis set, which is briefly described in the following section.. 2.1.7. Pseudo-potential method. Bl¨ och’s theorem defines an eigenfunction as,.

(34) 13. − n → ψ→ −(r ) =. X. k. → −. → −. → − → −. n, k i k . r c→ , − e. → − K. K. (2.10). → − → −. n, k where c→ are coefficients to be determined, ei k . r is a plane wave that contains the periodicity − K → − of the lattice, and k is a vector in the first Brillouin zone. Comparing Eqns. (2.9) and (2.10), we → − → − → − thus obtain that m represents (n, k ), and p represents ( k + K ). However, such a basis set is also. almost impossible to calculate accurately. Thus, the potential in regions close to the nuclei, which is its most fluctuating part, is replaced by a pseudo-potential that yields smooth wavefunctions near the atomic nucleus as this part of the solid behaves similarly to free atom electrons. This makes the basis set manageable to calculate for a system. Older pseudopotentials, such as norm-conserving [19] (where electron charge within the core part is equal to that of the actual atom) and ultrasoft [20, 21] pseudopotentials (do not conserve charge but reduce the heights of the peak in the potential that reduces the number of necessary plane waves) can be quite fast and accurate in some cases, and are still in use. The more recent projector augmented wave (PAW) method [18, 22–24] was used for the work presented in this thesis. Ref. [25] presents a comparison of the constructions and performances of these pseudopotentials methods. The PAW method involves the expansion of the wave functions in a plane wave basis set. It retains the full all-electron wave function and charge density while still being computationally efficient. Also, for plane waves, the cut-off can be easily set by limiting the set to k with k < Kmax .. 2.2. The CALPHAD method. The thermodynamics of solution phases is first described here as it forms the fundamental basis of the CALPHAD method. Solution is a term referred to a system in a solid, liquid or gaseous state, which exhibits solubility between the various components that make up the system. With relevance to the present work, thermodynamics of two-component systems or binary solutions will be dealt with in the following, noting that the formulation can be extended in a straightforward manner to ternary and higher-order systems..

(35) 14. 2.2.1. Ideal mixing. Ideal mixing represents an ideal case of no mixing or interactions in solutions. Statistical thermodynamics defines entropy in terms of disorder in the system. Kelvin and Boltzmann gave a mathematical formulation of this definition as:. S = k loge W,. (2.11). where k is Boltzmann’s constant and W is a measure of disorder in the system. If in a binary solution, out of a total of N sites n sites are occupied by A-type of atoms and the rest, (N − n) sites, by B-type atoms as shown in Fig. 2.1.. Figure 2.1: Schematic representation of random mixing of A and B atoms/molecules in a binary solution (adapted from Ref. [16]). The disorder or probability of distribution in this case is given by,. W =. N! . n!(N − n)!. (2.12). The entropy of this solution is then given by,. S = k loge. N! . n!(N − n)!. (2.13). After applying Stirling’s approximation and subsequent simplifications, the entropy change for ideal mixing is given by,. S = − R(xa loge xa + xb loge xb ).. (2.14). Thus, the Gibbs energy of mixing in case of no interactions between constitutive elements is given by,.

(36) 15. Gideal mix = RT (xa loge xa + xb loge xb ).. 2.2.2. (2.15). Non-ideal mixing. In reality, there is always some kind of interactions between different atom types in a solution. These interactions can either be attractive or repulsive in nature. The effects of such interactions are incorporated via the excess mixing energy term, Gxs mix , which is modeled in the simplest way according to the regular solution model:. Gxs mix = Ω xa xb ,. (2.16). where Ω is a regular solution parameter, and its sign depends on the nature of chemical interactions, positive for repulsive and negative for attractive interactions. The tendency to form a miscibility gap or two-phase structures in binary solution phases increases with an increase in magnitude of this regular solution parameter. In the case of attractive interactions or negative values of the regular solution parameter, the tendency is to form continuous solid solutions. Equations (2.15) and (2.16) combine to give the Gibbs energy of solution,. Gmix = RT (xa loge xb + xb loge xb ) + Ω xa xb .. (2.17). However, in the presence of crystallographically distinct phases, the Gibbs energy at end-points of the mixing curve have to be calculated, thus requiring that reference states be defined for the pure components. The Gibbs energy is then written as,. xs G = Gref + Gideal mix + Gmix ,. (2.18). where Gref is given by,. Gref =. X. xi Goi ,. (2.19). i. where xi is the mole fraction of component i, and Goi is the Gibbs energy of the phase for pure component i..

(37) 16. 2.2.3. Thermodynamic models. Solution phases are modeled via various methods, two of which are described here. 2.2.3.1. Random substitutional model. In this model, the components occupy crystal sites in a random manner rather than in an ordered manner, as shown in Fig. 2.2. Thus, gases, liquids and some metallic solid solutions are represented very well by this model.. Figure 2.2: Random occupation of sites on a bcc structure (adapted from Ref. [16]). In the present work, the liquid, and solid solution phases (that are non-stoichiometric) phases are modeled in this manner. One of the simplest non-ideal models is the regular solution model which considers no dependence of the nature of interactions between the components on the composition of the solution. The Gibbs free energy expression of such a model is given similar to Eqn. (2.18),. Gφm =. X. xi o Gφi + RT. i=A,B. X. xi loge xi + xA xB LφA,B ,. (2.20). i=A,B. where Gφm denotes the Gibbs energy of phase φ, xi is the mole fraction of component i, o Gφi defines the Gibbs energy of the phase containing the pure component i obtained from the SGTE database [26], and LφA,B is an interaction parameter that incorporates the effects of non-ideal mixing. To account for dependencies on changes in composition, this parameter is expanded using RedlichKister formalism [27] as, LφA,B =. X v. LφA,B (xA − xB )v .. (2.21).

(38) 17 The above equation for Gxs mix is considered a regular solution when v = 0 and non-regular solution when v > 1. Th binary interaction parameter is made temperature-dependent using,. v. LφA,B =. v. A +. v. BT,. (2.22). where v A and v B are model parameters to be optimized. 2.2.3.2. Sublattice model. This method of modeling phases can be applied to a variety of phase types such as interstitial and solution phases. The sublattice model can be visualized as consisting of interlocking sublattices as shown in Fig. 2.3.. Figure 2.3: A bcc structure shown with preferential occupation of sites by atoms on the two simple cubic sublattices (adapted from Ref. [16]). Its crystalline nature does not particularly represent a crystal structure within its general definition; however, certain external terms and conditions can be imposed to simulate special structure types. In this method it is necessary to define the fractional site occupation of each component in all the sublattices, which is given by,. s. yi =. nsi , Ns. (2.23). where nsi is the number of atoms of component i on sublattice s. In many cases, when vacancies are involved and become important to model a phase, such as an intermetallic phase, the site occupation is modified as,.

(39) 18. s. yi =. nsi nsV a +. X. nsi. ,. (2.24). i. where. nsV a. gives the number of vacancies on sublattice s. The Gibbs energy reference state is. obtained when only pure components can be considered as existing on each sublattice, and is given by,. Gref = m. X. PI0 (Y )o GφI0 ,. (2.25). I0. where PI0 represents the corresponding product of site fractions when each sublattice is occupied by only one component. In general, PIZ is the site fraction product when only one sublattice contains Z components and the remaining sublattices are occupied by one component. GφI0 is the Gibbs energy of the compound defined by I in phase φ. For example, if a two-sublattice phase is modeled as (A, B)1 (C, D)2 , where A, B, C and D are the components of this phase, the Gibbs energy reference state is written as,. Gref = yA yC GoAC + yA yD GoAD + yB yC GoBC + yB yD GoBD . m. (2.26). The ideal entropy of mixing in this case is given by,. Gideal mix = RT. X s. Ns. X. yis loge yis .. (2.27). i. Vacancies are included in the fractional site occupation term, yis . The ideal entropy term in the above expression includes all possible configuration contributions by all components mixing in each sublattice. The Gibbs excess energy of mixing for the two-sublattice system described previously as (A, B)1 (C, D)2 , is given by, 1 1 0 1 1 0 Gxs mix = yA yB LA,B:∗ + yC yD L∗:C,D .. (2.28). The above equation represents the regular solution format, and L0A,B:∗ and L0∗:C,D are the regular solution mixing parameters for each sublattice that are independent of the site occupation on the other sublattice. The sub-regular format includes the site occupation on the other sublattice as,.

(40) 19. 1 1 2 0 1 1 2 0 1 1 2 0 1 1 2 0 Gxs mix = yA yB yC LA,B:C + yA yB yD LA,B:D + yC yD yA LA:C,D + yC yD yB LB:C,D .. (2.29). Similar to the formalism in the case of the random solution model, the parameters are made composition dependent as,. 1 1 2 L0A,B:C = yA yB yC. X. 1 1 v LvA,B:C (yA − yB ) .. (2.30). v. The other parameters are modeled in a similar manner. The final Gibbs excess energy of mixing is given by,. Gxs mix =. XX. PIZ (Y )LφIZ .. (2.31). Z>0 IZ. Thus, the total Gibbs energy of this phase is obtained by combining the reference energy, ideal entropy contribution and excess energy contribution from Eqns. (2.25), (2.27), and (2.31), respectively, which is then given by,. Gφm =. X I0. 2.2.4. PI0 (Y )o GφI0 + RT. X s. Ns. X. s. yi loge s yi +. i. XX. PIZ (Y )LφIZ .. (2.32). Z>0 IZ. Evaluation of Gibbs energy parameters. After having made a decision of the model for the Gibbs energy of each phase to be considered for a given system, and entering all experimentally measured quantities and data from DFT calculations in an input file (.POP), the next step in the CALPHAD method is the evaluation of the parameters. This is carried out using an optimizer code that essentially revolves around Gibbs energy minimization. This type of code is based on the aim of reducing the statistical error between the experimental data and the calculated phase equilibria as much as possible..

(41) 20 2.2.4.1. Minimization procedure for single-phase equilibria. In the case of solution phases where enthalpies and entropies are temperature dependent, the Gibbs energy minimization is carried out by minimizing the function,. ∆G1φ =. X. φ. xφi Gi − Gφ = 0. (2.33). i. A Newton-Raphson method is used for rapid convergence. An initial temperature is chosen and both ∆G1φ and ∆G1φ /dT are calculated and then used to estimate a new temperature where ∆G1φ is expected to be equal to zero as shown in Fig. 2.4. If this new temperature does not satisfy the convergence condition, a new temperature is chosen. This process is repeated until ∆G1φ =0.. Figure 2.4: Schematic diagram showing the process of calculating the temperature at which ∆G1φ =0 (adapted from Ref. [16]).. 2.2.4.2. Minimization procedure for two-phase equilibria. The following mass balance equations will be utilized in the calculation of a two-phase equilibria,.

(42) 21. X. Niφ. (2.34). N i = M,. (2.35). Ni =. φ. and, X i. where Ni is the total number of mole of component i in the system, Nφi is the number of moles of component i in phase φ, and M is the total number of moles in the system.. The following is a brief description of the general minimization procedure: at first, the phase equilibrium is assumed to be single-phase. Then, an arbitrary amount of the second phase is introduced in the system, and in accordance with the mass balance equations a corresponding change is made in the composition of the first phase followed by the calculation of the Gibbs energy. The composition of this phase is then kept constant and the amount of the second phase is then varied with a corresponding change in its composition, to maintain mass balance, so that the Gibbs energy is minimized, as shown in Fig. 2.5.. Figure 2.5: First stage in the iteration process of Gibbs energy minimization of a Cu-Ni alloy at composition x0 in Cu, and at 1523 K (adapted from Ref. [16])..

(43) 22 The selection of the amount of the second phase to be varied can be made by calculating the second derivative of G with respect to Nliq to obtain the composition at which dG/dNliq =0, as shown in Figs. 2.6 and 2.7.. Figure 2.6: Gibbs energy versus N liq in an alloy shown schematically (adapted from Ref. [16]). This process is repeated until the Gibbs energy is minimized. The same procedure is then applied by varying the amount and composition of the first phase as shown in Fig. 2.8(a). This cycle is repeated as shown in Fig. 2.8(b) and 2.8(c) until a minimum is obtained in the Gibbs energy and the convergence criteria is satisfied. 2.2.4.3. Stepping and mapping. The previous procedures are for the calculation of equilibrium points at specific composition, temperature and pressure. However, for phase diagram calculations when changing a particular condition, such as composition or temperature in the present case, a procedure known as stepping is employed. In this process, a property is increased in small amounts or steps, and then the stability of the phase is checked at this step. If the phase is stable at that particular step, it is used as a starting point for the next step. This process is repeated until the conditions are not satisfied. Mapping is the process by which a phase diagram is plotted and employs the calculated results of the stepping code to map a phase boundary. Binary phase diagrams have two degrees of freedom that are most commonly represented by the temperature and composition..

(44) 23. Figure 2.7: Calculation of the second derivative of G with respect to N liq to obtain the minimum in Gibbs energy (adapted from Ref. [16]).. The requirements from a calculation method must be to reduce the degrees of freedom, calculate the Gibbs energy of the system, and use some iterative technique to minimize the Gibbs energy. Also, the robustness and the speed of the calculations depend heavily on the choice of starting guesses for the model parameters. Even though the calculation methods being used might be global minimization programs, there is always a possibility for the calculation to get stuck at a local minimum, thus giving an incorrect equilibrium result. Therefore, it is always recommended to have some prior knowledge of the phase diagram equilibria. This problem is most evident in the case of phases that have a miscibility gap. In case of availability of prior information on the miscibility information, such a phase is then given start points for both #1 and #2 phases (that form the miscibility gap) by the program and it ensures the convergence accounts for both minima. However, in a generalized environment, this method would fail if unknown miscibility gaps were present or if there was an order/disorder transition associated with the phase. Thus, some prior knowledge of miscibility gap or ordering is necessary to obtain reasonable accuracy and speed of execution..

(45) 24. (a). (b). (c). Figure 2.8: Second, third, and fourth stage in the iteration process of Gibbs energy minimization of a Cu-Ni alloy with composition x0 in Cu, and at 1523 K (adapted from Ref. [16]). 2.2.4.4. The PARROT programme. The PARROT module [28] is integrated with the Thermo-Calc package [29] and is essentially based on the following governing principles:. - Establish a criterion for best fit: This criterion is based on a maximum likelihood principle where a likelihood function is chosen and must be maximized to obtain the best estimates of the model parameters. Simplification of this process is made by assuming that the joint probability density function of all the experimental data is Gaussian in form, and that there is no dependence or coupling between different experimental measurements..